Characteristics and Availability of
Commercially Important Woods
Regis B. Miller
Timber Resources and Uses 1–2
Hardwoods and Softwoods 1–2
Commercial Sources of Wood Products 1–2
Use Classes and Trends 1–3
Species Descriptions 1–3
U.S. Wood Species 1–3
Imported Woods 1–17
hroughout history, the unique characteristics and
comparative abundance of wood have made it a
natural material for homes and other structures,
furniture, tools, vehicles, and decorative objects. Today, for
the same reasons, wood is prized for a multitude of uses.
All wood is composed of cellulose, lignin, hemicelluloses,
and minor amounts (5% to 10%) of extraneous materials
contained in a cellular structure. Variations in the characteristics
and volume of these components and differences in cellular
structure make woods heavy or light, stiff or flexible, and
hard or soft. The properties of a single species are relatively
constant within limits; therefore, selection of wood by species
alone may sometimes be adequate. However, to use
wood to its best advantage and most effectively in engineering
applications, specific characteristics or physical properties
must be considered.
Historically, some species filled many purposes, while other
less available or less desirable species served only one or two
needs. For example, because white oak is tough, strong, and
durable, it was highly prized for shipbuilding, bridges,
cooperage, barn timbers, farm implements, railroad crossties,
fence posts, and flooring. Woods such as black walnut and
cherry were used primarily for furniture and cabinets. Hickory
was manufactured into tough, hard, and resilient striking-tool
handles, and black locust was prized for barn timbers. What
the early builder or craftsman learned by trial and error became
the basis for deciding which species were appropriate
for a given use in terms of their characteristics. It was commonly
accepted that wood from trees grown in certain locations
under certain conditions was stronger, more durable,
more easily worked with tools, or finer grained than wood
from trees in other locations. Modern research on wood has
substantiated that location and growth conditions do
significantly affect wood properties.
The gradual reductions in use of old-growth forests in the
United States has reduced the supply of large clear logs for
lumber and veneer. However, the importance of high-quality
logs has diminished as new concepts of wood use have been
introduced. Second-growth wood, the remaining old-growth
forests, and imports continue to fill the needs for wood in the
quality required. Wood is as valuable an engineering material
as ever, and in many cases, technological advances have
made it even more useful.
The inherent factors that keep wood in the forefront of raw
materials are many and varied, but a chief attribute is its
availability in many species, sizes, shapes, and conditions to
suit almost every demand. Wood has a high ratio of strength
to weight and a remarkable record for durability and performance
as a structural material. Dry wood has good insulating
properties against heat, sound, and electricity. It tends to
absorb and dissipate vibrations under some conditions of
use, and yet it is an incomparable material for such musical
instruments as the violin. The grain patterns and colors of
wood make it an esthetically pleasing material, and its
appearance may be easily enhanced by stains, varnishes,
lacquers, and other finishes. It is easily shaped with tools
and fastened with adhesives, nails, screws, bolts, and dowels.
Damaged wood is easily repaired, and wood structures
are easily remodeled or altered. In addition, wood resists
oxidation, acid, saltwater, and other corrosive agents, has
high salvage value, has good shock resistance, can be treated
with preservatives and fire retardants, and can be combined
with almost any other material for both functional and
Timber Resources and Uses
In the United States, more than 100 wood species are available
to the prospective user, but all are unlikely to be available
in any one locality. About 60 native woods are of major
commercial importance. Another 30 species are commonly
imported in the form of logs, cants, lumber, and veneer for
industrial uses, the building trade, and crafts.
A continuing program of timber inventory is in effect in the
United States through the cooperation of Federal and State
agencies, and new information on wood resources is published
in State and Federal reports. Two of the most valuable
sourcebooks are An Analysis of the Timber Situation in the
United States 1989–2040 (USDA 1990) and The 1993 RPA
Timber Assessment Update (Haynes and others 1995).
Current information on wood consumption, production,
imports, and supply and demand is published periodically
by the Forest Products Laboratory (Howard 1997) and is
available from the Superintendent of Documents, U.S.
Government Printing Office, Washington, DC.
Hardwoods and Softwoods
Trees are divided into two broad classes, usually referred to
as hardwoods and softwoods. These names can be confusing
since some softwoods are actually harder than some hardwoods,
and conversely some hardwoods are softer than some
softwoods. For example, softwoods such as longleaf pine and
Douglas-fir are typically harder than the hardwoods basswood
and aspen. Botanically, hardwoods are Angiosperms; the
seeds are enclosed in the ovary of the flower. Anatomically,
hardwoods are porous; that is, they contain vessel elements.
A vessel element is a wood cell with open ends; when vessel
elements are set one above another, they form a continuous
tube (vessel), which serves as a conduit for transporting water
or sap in the tree. Typically, hardwoods are plants with
broad leaves that, with few exceptions in the temperate region,
lose their leaves in autumn or winter. Most imported
tropical woods are hardwoods. Botanically, softwoods are
Gymnosperms or conifers; the seeds are naked (not enclosed
in the ovary of the flower). Anatomically, softwoods are
nonporous and do not contain vessels. Softwoods are usually
cone-bearing plants with needle- or scale-like evergreen
leaves. Some softwoods, such as larches and baldcypress,
lose their needles during autumn or winter.
Major resources of softwood species are spread across the
United States, except for the Great Plains where only small
areas are forested. Softwood species are often loosely grouped
in three general regions, as shown in Table 1–1. Hardwoods
also occur in all parts of the United States, although most
grow east of the Great Plains. Hardwood species are shown
by region in Table 1–2.
of Wood Products
Softwoods are available directly from the sawmill, wholesale
and retail yards, or lumber brokers. Softwood lumber and
plywood are used in construction for forms, scaffolding,
framing, sheathing, flooring, moulding, paneling, cabinets,
poles and piles, and many other building components. Softwoods
may also appear in the form of shingles, sashes,
doors, and other millwork, in addition to some rough products
such as timber and round posts.
Hardwoods are used in construction for flooring, architectural
woodwork, interior woodwork, and paneling. These items
are usually available from lumberyards and building supply
dealers. Most hardwood lumber and dimension stock are
remanufactured into furniture, flooring, pallets, containers,
dunnage, and blocking. Hardwood lumber and dimension
Table 1–1. Major resources of U.S. softwoods according
Western Northern Southern
Incense-cedar Northern white-cedar Atlantic white-cedar
Port-Orford-cedar Balsam fir Baldcypress
Douglas-fir Eastern hemlock Fraser fir
White firs Fraser fir Southern Pine
Western hemlock Jack pine Eastern redcedar
Western larch Red pine
Lodgepole pine Eastern white pine
Ponderosa pine Eastern redcedar
Sugar pine Eastern spruces
Western white pine Tamarack
stock are available directly from the manufacturer, through
wholesalers and brokers, and from some retail yards.
Both softwood and hardwood products are distributed
throughout the United States. Local preferences and the
availability of certain species may influence choice, but a
wide selection of woods is generally available for building
construction, industrial uses, remanufacturing, and home use.
Use Classes and Trends
The production and consumption levels of some of the many
use-classifications for wood are increasing with the overall
national economy, and others are holding about the same.
The most vigorously growing wood-based industries are
those that convert wood to thin slices (veneer), particles
(chips, flakes), or fiber pulps and reassemble the elements to
produce various types of engineered panels such as plywood,
particleboard, strandboard, veneer lumber, paper, paperboard,
and fiberboard products. Another growing wood industry is
the production of laminated wood. For a number of years, the
lumber industry has produced almost the same volume of
wood per year. Modest increases have occurred in the production
of railroad crossties, cooperage, shingles, and shakes.
In this chapter, each species or group of species is described
in terms of its principal location, characteristics, and uses.
More detailed information on the properties of these and
other species is given in various tables throughout this
handbook. Information on historical and traditional uses is
provided for some species. Common and botanical names
follow the Checklist of United States Trees (Little 1979).
U.S. Wood Species
Red alder (Alnus rubra) grows along the Pacific coast between
Alaska and California. It is the principal hardwood for
commercial manufacture of wood products in Oregon and
Washington and the most abundant commercial hardwood
species in these two states.
The wood of red alder varies from almost white to pale
pinkish brown, and there is no visible boundary between
heartwood and sapwood. Red alder is moderately light in
weight and intermediate in most strength properties but low
in shock resistance. It has relatively low shrinkage.
The principal use of red alder is for furniture, but it is also
used for sash and door panel stock and other millwork.
Ash (White Ash Group)
Important species of the white ash group are American white
ash (Fraxinus americana), green ash (F. pennsylvanica), blue
ash (F. quadrangulata), and Oregon ash (F. latifolia). The
first three species grow in the eastern half of the United
States. Oregon ash grows along the Pacific Coast.
The heartwood of the white ash group is brown, and the
sapwood is light-colored or nearly white. Second-growth
trees are particularly sought after because of the inherent
qualities of the wood from these trees: it is heavy, strong,
hard, and stiff, and it has high resistance to shock. Oregon
ash has somewhat lower strength properties than American
white ash, but it is used for similar purposes on the West
American white ash is used principally for nonstriking tool
handles, oars, baseball bats, and other sporting and athletic
goods. For handles of the best grade, some handle specifications
call for not less than 2 nor more than 7 growth rings
per centimeter (not less than 5 nor more than 17 growth
rings per inch). The additional weight requirement of
690 kg/m3 (43 lb/ft3) or more at 12% moisture content ensures
high quality material. Principal uses for the white ash
group are decorative veneer, cabinets, furniture, flooring,
millwork, and crates.
Table 1–2. Major resources of U.S. hardwoods according
Ash Ash Red alder
Basswood Aspen Oregon ash
American beech Basswood Aspen
Butternut Buckeye Black cottonwood
Cottonwood Butternut California black oak
Elm American beech Oregon white oak
Hackberry Birch Bigleaf maple
Pecan hickory Black cherry Paper birch
True hickory American chestnuta Tanoak
Black locust Elm
Soft maple True hickory
Red oaks Honeylocust
White oaks Black locust
Sassafras Hard maple
Sweetgum Soft maple
American sycamore Red oaks
Tupelo White oaks
Black walnut American sycamore
Black willow Black walnut
aAmerican chestnut is no longer harvested, but chestnut
lumber from salvaged timbers can still be found on the
Ash (Black Ash Group)
The black ash group includes black ash (F. nigra) and
pumpkin ash (F. profunda). Black ash grows in the Northeast
and Midwest, and pumpkin ash in the South.
The heartwood of black ash is a darker brown than that of
American white ash; the sapwood is light-colored or nearly
white. The wood of the black ash group is lighter in weight
(basic specific gravity of 0.45 to 0.48) than that of the white
ash group (>0.50). Pumpkin ash, American white ash, and
green ash that grow in southern river bottoms, especially in
areas frequently flooded for long periods, produce buttresses
that contain relatively lightweight and brash wood.
Principal uses for the black ash group are decorative veneer,
cabinets, millwork, furniture, cooperage, and crates.
Aspen is a generally recognized name that is applied to
bigtooth (Populus grandidentata) and quaking
(P. tremuloides) aspen. Aspen does not include balsam
poplar (P. balsamifera) and the other species of Populus that
are included in the cottonwoods. In lumber statistics of the
U.S. Bureau of the Census, however, the term cottonwood
includes all the preceding species. Also, the lumber of aspen
and cottonwood may be mixed in trade and sold as either
popple or cottonwood. The name popple should not be
confused with yellow-poplar (Liriodendron tulipifera), also
known in the trade as poplar. Aspen lumber is produced
principally in the Northeastern and Lake States, with some
production in the Rocky Mountain States.
The heartwood of aspen is grayish white to light grayish
brown. The sapwood is lighter colored and generally merges
gradually into the heartwood without being clearly marked.
Aspen wood is usually straight grained with a fine, uniform
texture. It is easily worked. Well-dried aspen lumber does
not impart odor or flavor to foodstuffs. The wood of aspen is
lightweight and soft. It is low in strength, moderately stiff,
and moderately low in resistance to shock and has moderately
Aspen is cut for lumber, pallets, boxes and crating, pulpwood,
particleboard, strand panels, excelsior, matches, veneer,
and miscellaneous turned articles. Today, aspen is one
of the preferred species for use in oriented strandboard, a
panel product that is increasingly being used as sheathing.
American basswood (Tilia americana) is the most important
of the native basswood species; next in importance is white
basswood (T. heterophylla), and no attempt is made to
distinguish between these species in lumber form. In commercial
usage, ―white basswood‖ is used to specify the white
wood or sapwood of either species. Basswood grows in the
eastern half of the United States from the Canadian provinces
southward. Most basswood lumber comes from the Lake,
Middle Atlantic, and Central States.
The heartwood of basswood is pale yellowish brown with
occasional darker streaks. Basswood has wide, creamy white
or pale brown sapwood that merges gradually into heartwood.
When dry, the wood is without odor or taste. It is
soft and light in weight, has fine, even texture, and is
straight grained and easy to work with tools. Shrinkage in
width and thickness during drying is rated as high; however,
basswood seldom warps in use.
Basswood lumber is used mainly in venetian blinds, sashes
and door frames, moulding, apiary supplies, wooden ware,
and boxes. Some basswood is cut for veneer, cooperage,
excelsior, and pulpwood, and it is a favorite of wood carvers.
Only one species of beech, American beech (Fagus
grandifolia), is native to the United States. It grows in the
eastern one-third of the United States and adjacent Canadian
provinces. The greatest production of beech lumber is in the
Central and Middle Atlantic States.
In some beech trees, color varies from nearly white sapwood
to reddish-brown heartwood. Sometimes there is no clear
line of demarcation between heartwood and sapwood. Sapwood
may be roughly 7 to 13 cm (3 to 5 in.) wide. The
wood has little figure and is of close, uniform texture. It has
no characteristic taste or odor. The wood of beech is classed
as heavy, hard, strong, high in resistance to shock, and
highly suitable for steam bending. Beech shrinks substantially
and therefore requires careful drying. It machines
smoothly, is an excellent wood for turning, wears well, and
is rather easily treated with preservatives.
Most beech is used for flooring, furniture, brush blocks,
handles, veneer, woodenware, containers, and cooperage.
When treated with preservative, beech is suitable for
The three most important species are yellow birch (Betula
alleghaniensis), sweet birch (B. lenta), and paper birch
(B. papyrifera). These three species are the source of most
birch lumber and veneer. Other birch species of some commercial
importance are river birch (B. nigra), gray birch
(B. populifolia), and western paper birch (B. papyrifera var.
commutata). Yellow, sweet, and paper birch grow principally
in the Northeast and the Lake States; yellow and sweet birch
also grow along the Appalachian Mountains to northern
Yellow birch has white sapwood and light reddish-brown
heartwood. Sweet birch has light-colored sapwood and dark
brown heartwood tinged with red. For both yellow and sweet
birch, the wood is heavy, hard, and strong, and it has good
shock-resisting ability. The wood is fine and uniform in
texture. Paper birch is lower in weight, softer, and lower in
strength than yellow and sweet birch. Birch shrinks considerably
Yellow and sweet birch lumber is used primarily for the
manufacture of furniture, boxes, baskets, crates, wooden ware,
cooperage, interior woodwork, and doors; veneer plywood is
used for flush doors, furniture, paneling, cabinets, aircraft,
and other specialty uses. Paper birch is used for toothpicks,
tongue depressors, ice cream sticks, and turned products,
including spools, bobbins, small handles, and toys.
Buckeye consists of two species, yellow buckeye (Aesculus
octandra) and Ohio buckeye (A. glabra). These species
range from the Appalachians of Pennsylvania, Virginia, and
North Carolina westward to Kansas, Oklahoma, and Texas.
Buckeye is not customarily separated from other species
when manufactured into lumber and can be used for the same
purposes as aspen (Populus), basswood (Tilia), and sapwood
of yellow-poplar (Liriodendron tulipifera).
The white sapwood of buckeye merges gradually into the
creamy or yellowish white heartwood. The wood is uniform
in texture, generally straight grained, light in weight, weak
when used as a beam, soft, and low in shock resistance. It is
rated low on machinability such as shaping, mortising,
boring, and turning.
Buckeye is suitable for pulping for paper; in lumber form, it
has been used principally for furniture, boxes and crates,
food containers, wooden ware, novelties, and planing mill
Also called white walnut, butternut (Juglans cinerea) grows
from southern New Brunswick and Maine west to Minnesota.
Its southern range extends into northeastern Arkansas
and eastward to western North Carolina.
The narrow sapwood is nearly white and heartwood is light
brown, frequently modified by pinkish tones or darker brown
streaks. The wood is moderately light in weight (about the
same as eastern white pine), rather coarse textured, moderately
weak in bending and endwise compression, relatively
low in stiffness, moderately soft, and moderately high in
shock resistance. Butternut machines easily and finishes
well. In many ways, butternut resembles black walnut especially
when stained, but it does not have the same strength
Principal uses are for lumber and veneer, which are further
manufactured into furniture, cabinets, paneling, interior
woodwork, and miscellaneous rough items.
Black cherry (Prunus serotina) is sometimes known as
cherry, wild black cherry, and wild cherry. It is the only
native species of the genus Prunus of commercial importance
for lumber production. Black cherry is found from southeastern
Canada throughout the eastern half of the United States.
Production is centered chiefly in the Middle Atlantic States.
The heartwood of black cherry varies from light to dark
reddish brown and has a distinctive luster. The nearly white
sapwood is narrow in old-growth trees and wider in secondgrowth
trees. The wood has a fairly uniform texture and very
good machining properties. It is moderately heavy, strong,
stiff, and moderately hard; it has high shock resistance and
moderately high shrinkage. Black cherry is very dimensionally
stable after drying.
Black cherry is used principally for furniture, fine veneer
panels, and architectural woodwork. Other uses include
burial caskets, wooden ware, novelties, patterns, and
American chestnut (Castanea dentata) is also known as
sweet chestnut. Before this species was attacked by a blight
in the 1920s, it grew in commercial quantities from New
England to northern Georgia. Practically all standing chestnut
has been killed by blight, and most supplies of the
lumber come from salvaged timbers. Because of the species’
natural resistance to decay, standing dead trees in the Appalachian
Mountains continued to provide substantial quantities
of lumber for several decades after the blight, but this
source is now exhausted.
The heartwood of chestnut is grayish brown or brown and
darkens with age. The sapwood is very narrow and almost
white. The wood is coarse in texture; growth rings are made
conspicuous by several rows of large, distinct pores at the
beginning of each year’s growth. Chestnut wood is moderately
light in weight, moderately hard, moderately low in
strength, moderately low in resistance to shock, and low in
stiffness. It dries well and is easy to work with tools.
Chestnut was once used for poles, railroad crossties, furniture,
caskets, boxes, shingles, crates, and corestock for veneer
panels. At present, it appears most frequently as wormy
chestnut for paneling, interior woodwork, and picture frames.
Cottonwood includes several species of the genus Populus.
Most important are eastern cottonwood (P. deltoides and
varieties), also known as Carolina poplar and whitewood;
swamp cottonwood (P. heterophylla), also known as
cottonwood, river cottonwood, and swamp poplar; black
cottonwood (P. trichocarpa); and balsam poplar
(P. balsamifera). Eastern and swamp cottonwood grow
throughout the eastern half of the United States. Greatest
production of lumber is in the Southern and Central States.
Black cottonwood grows on the West Coast and in western
Montana, northern Idaho, and western Nevada. Balsam
poplar grows from Alaska across Canada and in the northern
Great Lakes States.
The heartwood of cottonwood is grayish white to light
brown. The sapwood is whitish and merges gradually with
the heartwood. The wood is comparatively uniform in texture
and generally straight grained. It is odorless when well
dried. Eastern cottonwood is moderately low in bending and
compressive strength, moderately stiff, moderately soft, and
moderately low in ability to resist shock. Most strength
properties of black cottonwood are slightly lower than those
of eastern cottonwood. Both eastern and black cottonwood
have moderately high shrinkage. Some cottonwood is
difficult to work with tools because of its fuzzy surface, which
is mainly the result of tension wood (see discussion of Reaction
Wood in Ch. 4).
Cottonwood is used principally for lumber, veneer, pulpwood,
excelsior, and fuel. Lumber and veneer are used
primarily for boxes, crates, baskets, and pallets.
Six species of elm grow in the eastern United States:
American (Ulmus americana), slippery (U. rubra), rock
(U. thomasii), winged (U. alata), cedar (U. crassifolia), and
September (U. serotina) elm. American elm is also known
as white, water, and gray elm; slippery elm as red elm; rock
elm as cork and hickory elm; winged elm as wahoo; cedar
elm as red and basket elm; and September elm as red elm.
American elm is threatened by two diseases, Dutch Elm
disease and phloem necrosis, which have killed hundreds of
thousands of trees.
Sapwood of elm is nearly white and heartwood light brown,
often tinged with red. Elm may be divided into two general
classes, soft and hard, based on the weight and strength of
the wood. Soft elm includes American and slippery elm. It is
moderately heavy, has high shock resistance, and is moderately
hard and stiff. Hard elm includes rock, winged, cedar,
and September elm. These species are somewhat heavier than
soft elm. Elm has excellent bending qualities.
Historically, elm lumber was used for boxes, baskets, crates,
and slack cooperage; furniture; agricultural supplies and
implements; caskets and burial boxes; and wood components
in vehicles. Today, elm lumber and veneer are used mostly
for furniture and decorative panels. Hard elm is preferred for
uses that require strength.
Hackberry (Celtis occidentalis) and sugarberry (C. laevigata)
supply the lumber known in the trade as hackberry. Hackberry
grows east of the Great Plains from Alabama, Georgia,
Arkansas, and Oklahoma northward, except along the Canadian
boundary. Sugarberry overlaps the southern part of the
hackberry range and grows throughout the Southern and
South Atlantic States.
Sapwood of both species varies from pale yellow to greenish
or grayish yellow. The heartwood is commonly darker. The
wood resembles elm in structure. Hackberry lumber is moderately
heavy. It is moderately strong in bending, moderately
weak in compression parallel to grain, moderately hard to
very hard, and high in shock resistance, but low in stiffness.
Hackberry has high shrinkage but keeps its shape well during
Most hackberry is cut into lumber; small amounts are used
for furniture parts, dimension stock, and veneer.
Hickory (Pecan Group)
Species of the pecan hickory group include bitternut hickory
(Carya cordiformis), pecan (C. illinoensis), water hickory
(C. aquatica), and nutmeg hickory (C. myristiciformis).
Bitternut hickory grows throughout the eastern half of the
United States; pecan hickory, from central Texas and
Louisiana to Missouri and Indiana; water hickory, from
Texas to South Carolina; and nutmeg hickory, in Texas
The sapwood of this group is white or nearly white and
relatively wide. The heartwood is somewhat darker. The
wood is heavy and sometimes has very high shrinkage.
Heavy pecan hickory is used for tool and implement handles
and flooring. The lower grades are used for pallets. Many
higher grade logs are sliced to provide veneer for furniture
and decorative paneling.
Hickory (True Group)
True hickories are found throughout the eastern half of the
United States. The species most important commercially are
shagbark (Carya ovata), pignut (C. glabra), shellbark
(C. laciniosa), and mockernut (C. tomentosa). The greatest
commercial production of the true hickories for all uses is in
the Middle Atlantic and Central States, with the Southern
and South Atlantic States rapidly expanding to handle nearly
half of all hickory lumber.
The sapwood of the true hickory group is white and usually
quite wide, except in old, slow-growing trees. The heartwood
is reddish. The wood is exceptionally tough, heavy,
hard, and strong, and shrinks considerably in drying. For
some purposes, both rings per centimeter (or inch) and
weight are limiting factors where strength is important.
The major use for high quality hickory is for tool handles,
which require high shock resistance. It is also used for ladder
rungs, athletic goods, agricultural implements, dowels,
gymnasium apparatuses, poles, and furniture. Lower grade
hickory is not suitable for the special uses of high quality
hickory because of knottiness or other growth features and
low density. However, the lower grade is useful for pallets
and similar items. Hickory sawdust, chips, and some solid
wood are used to flavor meat by smoking.
The wood of honeylocust (Gleditsia triacanthos) has many
desirable qualities, such as attractive figure and color, hardness,
and strength, but it is little used because of its scarcity.
Although the natural range of honeylocust has been extended
by planting, this species is found most commonly in the
eastern United States, except for New England and the South
Atlantic and Gulf Coastal Plains.
Sapwood is generally wide and yellowish, in contrast to the
light red to reddish-brown heartwood. The wood is very
heavy, very hard, strong in bending, stiff, resistant to shock,
and durable when in contact with the ground.
When available, honeylocust is primarily used locally for
fence posts and general construction. It is occasionally used
with other species in lumber for pallets and crating.
Black locust (Robinia pseudoacacia) is sometimes called
yellow or post locust. This species grows from Pennsylvania
along the Appalachian Mountains to northern Georgia and
Alabama. It is also native to western Arkansas and southern
Missouri. The greatest production of black locust timber is
in Tennessee, Kentucky, West Virginia, and Virginia.
Locust has narrow, creamy white sapwood. The heartwood,
when freshly cut, varies from greenish yellow to dark brown.
Black locust is very heavy, very hard, very resistant to
shock, and very strong and stiff. It has moderately low
shrinkage. The heartwood has high decay resistance.
Black locust is used for round, hewed, or split mine timbers
as well as fence posts, poles, railroad crossties, stakes, and
fuel. Other uses are for rough construction, crating, and mine
equipment. Historically, black locust was important for the
manufacture of insulator pins and wooden pegs used in the
construction of ships, for which the wood was well adapted
because of its strength, decay resistance, and moderate
shrinkage and swelling.
Commercial magnolia consists of three species: southern
magnolia (Magnolia grandiflora), sweetbay (M. virginiana),
and cucumbertree (M. acuminata). Other names for southern
magnolia are evergreen magnolia, big laurel, bull bay, and
laurel bay. Sweetbay is sometimes called swamp magnolia.
The lumber produced by all three species is simply called
magnolia. The natural range of sweetbay extends along the
Atlantic and Gulf Coasts from Long Island to Texas, and
that of southern magnolia extends from North Carolina to
Texas. Cucumbertree grows from the Appalachians to the
Ozarks northward to Ohio. Louisiana leads in the production
of magnolia lumber.
Sapwood of southern magnolia is yellowish white, and
heartwood is light to dark brown with a tinge of yellow or
green. The wood, which has close, uniform texture and is
generally straight grained, closely resembles yellow-poplar
(Liriodendron tulipifera). It is moderately heavy, moderately
low in shrinkage, moderately low in bending and compressive
strength, moderately hard and stiff, and moderately high
in shock resistance. Sweetbay is much like southern magnolia.
The wood of cucumbertree is similar to that of yellowpoplar
(L. tulipifera); cucumbertree that grows in the yellowpoplar
range is not separated from that species on the market.
Magnolia lumber is used principally in the manufacture of
furniture, boxes, pallets, venetian blinds, sashes, doors,
veneer, and millwork.
Hard maple includes sugar maple (Acer saccharum) and
black maple (A. nigrum). Sugar maple is also known as hard
and rock maple, and black maple as black sugar maple.
Maple lumber is manufactured principally in the Middle
Atlantic and Great Lake States, which together account for
about two-thirds of production.
The heartwood is usually light reddish brown but sometimes
considerably darker. The sapwood is commonly white with a
slight reddish-brown tinge. It is roughly 7 to 13 cm or more
(3 to 5 in. or more) wide. Hard maple has a fine, uniform
texture. It is heavy, strong, stiff, hard, and resistant to shock
and has high shrinkage. The grain of sugar maple is generally
straight, but birdseye, curly, or fiddleback grain is often
selected for furniture or novelty items.
Hard maple is used principally for lumber and veneer. A
large proportion is manufactured into flooring, furniture,
cabinets, cutting boards and blocks, pianos, billiard cues,
handles, novelties, bowling alleys, dance and gymnasium
floors, spools, and bobbins.
Soft maple includes silver maple (Acer saccharinum), red
maple (A. rubrum), boxelder (A. negundo), and bigleaf maple
(A. macrophyllum). Silver maple is also known as white,
river, water, and swamp maple; red maple as soft, water,
scarlet, white, and swamp maple; boxelder as ash-leaved,
three-leaved, and cut-leaved maple; and bigleaf maple as
Oregon maple. Soft maple is found in the eastern United
States except for bigleaf maple, which comes from the
Heartwood and sapwood are similar in appearance to hard
maple: heartwood of soft maple is somewhat lighter in color
and the sapwood, somewhat wider. The wood of soft maple,
primarily silver and red maple, resembles that of hard maple
but is not as heavy, hard, and strong.
Soft maple is used for railroad crossties, boxes, pallets,
crates, furniture, veneer, wooden ware, and novelties.
Oak (Red Oak Group)
Most red oak comes from the Eastern States. The principal
species are northern red (Quercus rubra), scarlet (Q. coccinea),
Shumard (Q. shumardii), pin (Q. palustris), Nuttall
(Q. nuttallii), black (Q. velutina), southern red (Q. falcata),
cherrybark (Q. falcata var. pagodaefolia), water (Q. nigra),
laurel (Q. laurifolia), and willow (Q. phellos) oak.
The sapwood is nearly white and roughly 2 to 5 cm
(1 to 2 in.) wide. The heartwood is brown with a tinge of
red. Sawn lumber of the red oak group cannot be separated
by species on the basis of wood characteristics alone.
Red oak lumber can be separated from white oak by the size
and arrangement of pores in latewood and because it generally
lacks tyloses in the pores. The open pores of red oak
make this species group unsuitable for tight cooperage,
unless the barrels are lined with sealer or plastic. Quartersawn
lumber of the oaks is distinguished by the broad and
conspicuous rays. Wood of the red oaks is heavy. Rapidly
grown second-growth wood is generally harder and tougher
than finer textured old-growth wood. The red oaks have fairly
high shrinkage in drying.
The red oaks are primarily cut into lumber, railroad crossties,
mine timbers, fence posts, veneer, pulpwood, and
fuelwood. Ties, mine timbers, and fence posts require preservative
treatment for satisfactory service. Red oak lumber is
remanufactured into flooring, furniture, general millwork,
boxes, pallets and crates, agricultural implements, caskets,
wooden ware, and handles. It is also used in railroad cars
Oak (White Oak Group)
White oak lumber comes chiefly from the South, South
Atlantic, and Central States, including the southern Appalachian
area. Principal species are white (Quercus alba), chestnut
(Q. prinus), post (Q. stellata), overcup (Q. lyrata),
swamp chestnut (Q. michauxii), bur (Q. macrocarpa),
chinkapin (Q. muehlenbergii), swamp white (Q. bicolor),
and live (Q. virginiana) oak.
The sapwood of the white oaks is nearly white and roughly
2 to 5 cm or more (1 to 2 in. or more) wide. The heartwood
is generally grayish brown. Heartwood pores are usually
plugged with tyloses, which tend to make the wood impenetrable
by liquids. Consequently, most white oaks are suitable
for tight cooperage. Many heartwood pores of chestnut
oak lack tyloses. The wood of white oak is heavy, averaging
somewhat greater in weight than red oak wood. The heartwood
has good decay resistance.
White oaks are usually cut into lumber, railroad crossties,
cooperage, mine timbers, fence posts, veneer, fuelwood, and
many other products. High-quality white oak is especially
sought for tight cooperage. Live oak is considerably heavier
and stronger than the other oaks, and it was formerly used
extensively for ship timbers. An important use of white oak
is for planking and bent parts of ships and boats; heartwood
is often specified because of its decay resistance. White oak is
also used for furniture, flooring, pallets, agricultural implements,
railroad cars, truck floors, furniture, doors, and
Sassafras (Sassafras albidum) ranges through most of the
eastern half of the United States, from southeastern Iowa and
eastern Texas eastward.
Sassafras is easily confused with black ash, which it resembles
in color, grain, and texture. Sapwood is light yellow,
and heartwood varies from dull grayish brown to dark brown,
sometimes with a reddish tinge. Freshly cut surfaces have the
characteristic odor of sassafras. The wood is moderately
heavy, moderately hard, moderately weak in bending and
endwise compression, quite high in shock resistance, and
resistant to decay.
Sassafras was highly prized by the Indians for dugout canoes,
and some sassafras lumber is still used for small boats.
Locally, sassafras is used for fence posts and rails and for
Sweetgum (Liquidambar styraciflua) grows from southwestern
Connecticut westward into Missouri and southward to
the Gulf Coast. Almost all lumber is produced in the Southern
and South Atlantic States.
The lumber from sweetgum is usually marked as sap gum
(the light-colored sapwood) or redgum (the reddish-brown
heartwood). Sweetgum often has a form of cross grain called
interlocked grain, and it must be dried slowly. When quartersawn,
interlocked grain produces a ribbon-type stripe that
is desirable for interior woodwork and furniture. The wood is
moderately heavy and hard. It is moderately strong, moderately
stiff, and moderately high in shock resistance.
Sweetgum is used principally for lumber, veneer, plywood,
slack cooperage, railroad crossties, fuel, pulpwood, boxes
and crates, furniture, interior moulding, and millwork.
American sycamore (Platanus occidentalis) is known as
sycamore and sometimes as buttonwood, buttonball-tree, and
in the United Kingdom, planetree. Sycamore grows from
Maine to Nebraska, southward to Texas, and eastward to
The heartwood of sycamore is reddish brown; the sapwood is
lighter in color and from 4 to 8 cm (1-1/2 to 3 in.) wide.
The wood has a fine texture and interlocked grain. It has
high shrinkage in drying; is moderately heavy, moderately
hard, moderately stiff, and moderately strong; and has good
resistance to shock.
Sycamore is used principally for lumber, veneer, railroad
crossties, slack cooperage, fence posts, and fuel. The lumber
is used for furniture, boxes (particularly small food containers),
pallets, flooring, handles, and butcher blocks. Veneer is
used for fruit and vegetable baskets and some decorative
panels and door skins.
Tanoak (Lithocarpus densiflorus) has recently gained some
commercial value, primarily in California and Oregon. It is
also known as tanbark–oak because high-grade tannin was
once obtained from the bark in commercial quantities. This
species is found in southwestern Oregon and south to
Southern California, mostly near the coast but also in the
Sapwood of tanoak is light reddish brown when first cut and
turns darker with age to become almost indistinguishable
from heartwood, which also ages to dark reddish brown. The
wood is heavy and hard; except for compression perpendicular
to grain, the wood has roughly the same strength properties
as those of eastern white oak. Tanoak has higher shrinkage
during drying than does white oak, and it has a tendency
to collapse during drying. Tanoak is quite susceptible to
decay, but the sapwood takes preservatives easily. Tanoak
has straight grain, machines and glues well, and takes stains
Because of its hardness and abrasion resistance, tanoak is
excellent for flooring in homes or commercial buildings.
It is also suitable for industrial applications such as truck
flooring. Tanoak treated with preservative has been used for
railroad crossties. The wood has been manufactured into
baseball bats with good results, and it is also suitable for
veneer, both decorative and industrial, and for high quality
The tupelo group includes water (Nyssa aquatica), black
(N. sylvatica), swamp (N. sylvatica var. biflora), and
Ogeechee (N. ogeche) tupelo. Water tupelo is also known as
tupelo gum, swamp tupelo, and sourgum; black tupelo, as
blackgum and sourgum; swamp tupelo, as swamp blackgum,
blackgum, and sourgum; and Ogeechee tupelo, as sour tupelo,
gopher plum, and Ogeechee plum. All except black
tupelo grow principally in the southeastern United States.
Black tupelo grows in the eastern United States from Maine
to Texas and Missouri. About two-thirds of the production
of tupelo lumber is from Southern States.
Wood of the different tupelo species is quite similar in
appearance and properties. The heartwood is light brownish
gray and merges gradually into the lighter-colored sapwood,
which is generally many centimeters wide. The wood has
fine, uniform texture and interlocked grain. Tupelo wood is
moderately heavy, moderately strong, moderately hard and
stiff, and moderately high in shock resistance. Buttresses of
trees growing in swamps or flooded areas contain wood that
is much lighter in weight than that from upper portions of
the same trees. Because of interlocked grain, tupelo lumber
requires care in drying.
Tupelo is cut principally for lumber, veneer, pulpwood, and
some railroad crossties and slack cooperage. Lumber goes
into boxes, pallets, crates, baskets, and furniture.
Black walnut (Juglans nigra), also known as American black
walnut, ranges from Vermont to the Great Plains and southward
into Louisiana and Texas. About three-quarters of
walnut wood is grown in the Central States.
The heartwood of black walnut varies from light to dark
brown; the sapwood is nearly white and up to 8 cm (3 in.)
wide in open-grown trees. Black walnut is normally straight
grained, easily worked with tools, and stable in use. It is
heavy, hard, strong, and stiff, and has good resistance to
shock. Black walnut is well suited for natural finishes.
Because of its good properties and interesting grain pattern,
black walnut is much valued for furniture, architectural
woodwork, and decorative panels. Other important uses are
gunstocks, cabinets, and interior woodwork.
Black willow (Salix nigra) is the most important of the
many willows that grow in the United States. It is the only
willow marketed under its own name. Most black willow
comes from the Mississippi Valley, from Louisiana to southern
Missouri and Illinois.
The heartwood of black willow is grayish brown or light
reddish brown and frequently contains darker streaks. The
sapwood is whitish to creamy yellow. The wood is uniform
in texture, with somewhat interlocked grain, and light in
weight. It has exceedingly low strength as a beam or post, is
moderately soft, and is moderately high in shock resistance.
It has moderately high shrinkage.
Black willow is principally cut into lumber. Small amounts
are used for slack cooperage, veneer, excelsior, charcoal,
pulpwood, artificial limbs, and fence posts. The lumber is
remanufactured principally into boxes, pallets, crates, caskets,
Yellow-poplar (Liriodendron tulipifera) is also known as
poplar, tulip-poplar, and tulipwood. Sapwood from yellowpoplar
is sometimes called white poplar or whitewood.
Yellow-poplar grows from Connecticut and New York
southward to Florida and westward to Missouri. The greatest
commercial production of yellow-poplar lumber is in the
South and Southeast.
Yellow-poplar sapwood is white and frequently several centimeters
wide. The heartwood is yellowish brown, sometimes
streaked with purple, green, black, blue, or red. These
colorations do not affect the physical properties of the wood.
The wood is generally straight grained and comparatively
uniform in texture. Slow-grown wood is moderately light in
weight and moderately low in bending strength, moderately
soft, and moderately low in shock resistance. The wood has
moderately high shrinkage when dried from a green condition,
but it is not difficult to dry and is stable after drying.
Much of the second-growth wood is heavier, harder, and
stronger than that of older trees that have grown more
The lumber is used primarily for furniture, interior moulding,
siding, cabinets, musical instruments, and structural
components. Boxes, pallets, and crates are made from lowergrade
stock. Yellow-poplar is also made into plywood for
paneling, furniture, piano cases, and various other special
Baldcypress or cypress (Taxodium distichum) is also known
as southern-cypress, red-cypress, yellow-cypress, and whitecypress.
Commercially, the terms tidewater red-cypress, gulfcypress,
red-cypress (coast type), and yellow-cypress (inland
type) are frequently used. About half of the cypress lumber
comes from the Southern States and about a fourth from the
South Atlantic States (Fig. 1–1). Old-growth baldcypress is
no longer readily available, but second-growth wood is
Sapwood of baldcypress is narrow and nearly white. The
color of heartwood varies widely, ranging from light yellowish
brown to dark brownish red, brown, or chocolate.
The wood is moderately heavy, moderately strong, and
moderately hard. The heartwood of old-growth baldcypress
is one of the most decay resistant of U.S. species, but secondgrowth wood is only moderately resistant to decay.
Shrinkage is moderately low but somewhat higher than that
of the cedars and lower than that of Southern Pine. The wood
of certain baldcypress trees frequently contains pockets or
localized areas that have been attacked by a fungus. Such
wood is known as pecky cypress. The decay caused by this
fungus is stopped when the wood is cut into lumber and
dried. Pecky cypress is therefore durable and useful where
water tightness is unnecessary, appearance is not important,
or a novel effect is desired.
When old-growth wood was available, baldcypress was used
principally for building construction, especially where resistance
to decay was required. It was also used for caskets,
sashes, doors, blinds, tanks, vats, ship and boat building,
and cooling towers. Second-growth wood is used for siding
and millwork, including interior woodwork and paneling.
Pecky cypress is used for paneling in restaurants, stores, and
Douglas-fir (Pseudotsuga menziesii) is also known locally as
red-fir, Douglas-spruce, and yellow-fir. Its range extends from
the Rocky Mountains to the Pacific Coast and from Mexico
to central British Columbia.
Sapwood of Douglas-fir is narrow in old-growth trees but
may be as much as 7 cm (3 in.) wide in second-growth trees
of commercial size. Young trees of moderate to rapid growth
have reddish heartwood and are called red-fir. Very narrowringed
heartwood of old-growth trees may be yellowish
brown and is known on the market as yellow-fir. The wood
of Douglas-fir varies widely in weight and strength. When
lumber of high strength is needed for structural uses, selection
can be improved by selecting wood with higher density.
Douglas-fir is used mostly for building and construction
purposes in the form of lumber, marine fendering (Fig. 1–2),
piles, and plywood. Considerable quantities are used for
railroad crossties, cooperage stock, mine timbers, poles, and
fencing. Douglas-fir lumber is used in the manufacture of
various products, including sashes, doors, laminated beams,
general millwork, railroad-car construction, boxes, pallets,
and crates. Small amounts are used for flooring, furniture,
ship and boat construction, and tanks. Douglas-fir plywood
has found application in construction, furniture, cabinets,
marine use, and other products.
Firs, True (Eastern Species)
Balsam fir (Abies balsamea) grows principally in New England,
New York, Pennsylvania, and the Great Lake States.
Fraser fir (A. fraseri) grows in the Appalachian Mountains of
Virginia, North Carolina, and Tennessee.
The wood of the eastern true firs, as well as the western true
firs, is creamy white to pale brown. The heartwood and
sapwood are generally indistinguishable. The similarity of
wood structure in the true firs makes it impossible to distinguish
the species by examination of the wood alone. Balsam
and Fraser firs are lightweight, have low bending and compressive
strength, are moderately low in stiffness, are soft,
and have low resistance to shock.
The eastern firs are used mainly for pulpwood, although
some lumber is produced for structural products, especially
in New England and the Great Lake States.
Firs, True (Western Species)
Six commercial species make up the western true firs: subalpine
fir (Abies lasiocarpa), California red fir (A. magnifica),
grand fir (A. grandis), noble fir (A. procera), Pacific silver fir
(A. amabilis), and white fir (A. concolor). The western true
firs are cut for lumber primarily in Washington, Oregon,
California, western Montana, and northern Idaho, and they
are marketed as white fir throughout the United States.
Figure 1–1. Cypress-tupelo swamp near New Orleans,
LA. Species include baldcypress (Taxodium distichum)),
tupelo (Nyssa), ash (Fraxinus), willow (Salix), and elm
(Ulmus). Swollen buttresses and “knees” are typically
present in cypress.
The wood of the western true firs is similar to that of the
eastern true firs, which makes it impossible to distinguish
the true fir species by examination of the wood alone. Western
true firs are light in weight but, with the exception of
subalpine fir, have somewhat higher strength properties than
does balsam fir. Shrinkage of the wood is low to moderately
Lumber of the western true firs is primarily used for building
construction, boxes and crates, planing-mill products,
sashes, doors, and general millwork. In house construction,
the lumber is used for framing, subflooring, and sheathing.
Some western true fir lumber is manufactured into boxes and
crates. High-grade lumber from noble fir is used mainly for
interior woodwork, moulding, siding, and sash and door
stock. Some of the highest quality material is suitable for
aircraft construction. Other special uses of noble fir are venetian
blinds and ladder rails.
Eastern hemlock (Tsuga canadensis) grows from New England
to northern Alabama and Georgia, and in the Great Lake
States. Other names are Canadian hemlock and hemlock–
spruce. The production of hemlock lumber is divided fairly
evenly among the New England States, Middle Atlantic
States, and Great Lake States.
The heartwood of eastern hemlock is pale brown with a
reddish hue. The sapwood is not distinctly separated from
the heartwood but may be lighter in color. The wood is
coarse and uneven in texture (old trees tend to have considerable
shake); it is moderately lightweight, moderately hard,
moderately low in strength, moderately stiff, and moderately
low in shock resistance.
Eastern hemlock is used principally for lumber and pulpwood.
The lumber is used primarily in building construction
(framing, sheathing, subflooring, and roof boards) and in the
manufacture of boxes, pallets, and crates.
Figure 1–2. Wood is favored for waterfront structures, particularly fendering, because of its shockabsorbing qualities.
The fendering on this dock in Key West, FL, is made of creosote-treated Douglas-fir (Pseudotsuga
tropical species are resistant to attack by decay fungi and marine borers and are used for marine
without preservative treatment.
Hemlock, Western and Mountain
Western hemlock (Tsuga heterophylla) is also known as
West Coast hemlock, Pacific hemlock, British Columbia
hemlock, hemlock–spruce, and western hemlock–fir. It grows
along the Pacific coast of Oregon and Washington and in the
northern Rocky Mountains north to Canada and Alaska. A
relative of western hemlock, mountain hemlock (T. mertensiana)
grows in mountainous country from central California
to Alaska. It is treated as a separate species in assigning
The heartwood and sapwood of western hemlock are almost
white with a purplish tinge. The sapwood, which is sometimes
lighter in color than the heartwood, is generally not
more than 2.5 cm (1 in.) wide. The wood often contains
small, sound, black knots that are usually tight and dimensionally
stable. Dark streaks are often found in the lumber;
these are caused by hemlock bark maggots and generally do
not reduce strength. Western hemlock is moderately light in
weight and moderate in strength. It is also moderate in
hardness, stiffness, and shock resistance. Shrinkage of western
hemlock is moderately high, about the same as that of
Douglas-fir (Pseudotsuga menziesii). Green hemlock lumber
contains considerably more water than does Douglas-fir and
requires longer kiln-drying time. Mountain hemlock has
approximately the same density as that of western hemlock
but is somewhat lower in bending strength and stiffness.
Western hemlock and mountain hemlock are used principally
for pulpwood, lumber, and plywood. The lumber is used
primarily for building material, such as sheathing, siding,
subflooring, joists, studding, planking, and rafters, as well as
in the manufacture of boxes, pallets, crates, flooring, furniture,
Incense-cedar (Calocedrus decurrens (synonym Libocedrus
decurrens)) grows in California, southwestern Oregon, and
extreme western Nevada. Most incense-cedar lumber comes
from the northern half of California.
Sapwood of incense-cedar is white or cream colored, and
heartwood is light brown, often tinged with red. The wood
has a fine, uniform texture and a spicy odor. Incense-cedar is
light in weight, moderately low in strength, soft, low in
shock resistance, and low in stiffness. It has low shrinkage
and is easy to dry, with little checking or warping.
Incense-cedar is used principally for lumber and fence posts.
Nearly all the high-grade lumber is used for pencils and
venetian blinds; some is used for chests and toys. Much
incense-cedar wood is more or less pecky; that is, it contains
pockets or areas of disintegrated wood caused by advanced
stages of localized decay in the living tree. There is no further
development of decay once the lumber is dried. This
low-quality lumber is used locally for rough construction
where low cost and decay resistance are important. Because
of its resistance to decay, incense-cedar is well suited for
fence posts. Other uses are railroad crossties, poles, and split
Western larch (Larix occidentalis) grows in western Montana,
northern Idaho, northeastern Oregon, and on the eastern
slope of the Cascade Mountains in Washington. About twothirds
of the lumber of this species is produced in Idaho and
Montana and one-third in Oregon and Washington.
The heartwood of western larch is yellowish brown and the
sapwood, yellowish white. The sapwood is generally not
more than 2.5 cm (1 in.) wide. The wood is stiff, moderately
strong and hard, moderately high in shock resistance, and
moderately heavy. It has moderately high shrinkage. The
wood is usually straight grained, splits easily, and is subject
to ring shake. Knots are common but generally small and
Western larch is used mainly for rough dimension wood in
building construction, small timbers, planks and boards, and
railroad crossties and mine timbers. It is used also for piles,
poles, and posts. Some high-grade material is manufactured
into interior woodwork, flooring, sashes, and doors. The
properties of western larch are similar to those of Douglas-fir
(Pseudotsuga menziesii), and these species are sometimes
Pine, Eastern White
Eastern white pine (Pinus strobus) grows from Maine to
northern Georgia and in the Great Lake States. It is also
known as white pine, northern white pine, Weymouth pine,
and soft pine. About one-half the production of eastern white
pine lumber occurs in New England, about one-third in the
Great Lake States, and most of the remainder in the Middle
Atlantic and South Atlantic States.
The heartwood of eastern white pine is light brown, often
with a reddish tinge. It turns darker on exposure to air. The
wood has comparatively uniform texture and is straight
grained. It is easily kiln dried, has low shrinkage, and ranks
high in stability. It is also easy to work and can be readily
glued. Eastern white pine is lightweight, moderately soft,
moderately low in strength, low in shock resistance, and low
Practically all eastern white pine is converted into lumber,
which is used in a great variety of ways. A large proportion,
mostly second-growth knotty wood or lower grades, is used
for structural lumber. High-grade lumber is used for patterns
for castings. Other important uses are sashes, doors, furniture,
interior woodwork, knotty paneling, caskets, shade and
map rollers, and toys.
Jack pine (Pinus banksiana), sometimes known as scrub,
gray, and black pine in the United States, grows naturally in
the Great Lake States and in a few scattered areas in New
England and northern New York. Jack pine lumber is sometimes
not separated from the other pines with which it
grows, including red pine (Pinus resinosa) and eastern white
pine (Pinus strobus).
Sapwood of jack pine is nearly white; heartwood is light
brown to orange. Sapwood may constitute one-half or more
of the volume of a tree. The wood has a rather coarse texture
and is somewhat resinous. It is moderately lightweight,
moderately low in bending strength and compressive
strength, moderately low in shock resistance, and low in
stiffness. It also has moderately low shrinkage. Lumber from
jack pine is generally knotty.
Jack pine is used for pulpwood, box lumber, and pallets.
Less important uses include railroad crossties, mine timber,
slack cooperage, poles, posts, and fuel.
Pine, Jeffrey (see Pine, Ponderosa)
Lodgepole pine (Pinus contorta), also known as knotty,
black, and spruce pine, grows in the Rocky Mountain and
Pacific Coast regions as far northward as Alaska. Wood for
lumber and other products is produced primarily in the
central Rocky Mountain States; other producing regions are
Idaho, Montana, Oregon, and Washington.
The heartwood of lodgepole pine varies from light yellow to
light yellow-brown. The sapwood is yellow or nearly white.
The wood is generally straight grained with narrow growth
rings. The wood is moderately lightweight, is fairly easy to
work, and has moderately high shrinkage. It is moderately
low in strength, moderately soft, moderately stiff, and moderately
low in shock resistance.
Lodgepole pine is used for lumber, mine timbers, railroad
crossties, and poles. Less important uses include posts and
fuel. Lodgepole pine is being used increasingly for framing,
siding, millwork, flooring, and cabin logs.
Pitch pine (Pinus rigida) grows from Maine along the mountains
to eastern Tennessee and northern Georgia.
The heartwood is brownish red and resinous; the sapwood is
wide and light yellow. The wood of pitch pine is moderately
heavy to heavy, moderately strong, stiff, and hard, and
moderately high in shock resistance. Shrinkage ranges from
moderately low to moderately high.
Pitch pine is used for lumber, fuel, and pulpwood. The
lumber is classified as a minor species in grading rules for
the Southern Pine species group.
Pond pine (Pinus serotina) grows in the coastal region from
New Jersey to Florida. It occurs in small groups or singly,
mixed with other pines on low flats.
Sapwood of pond pine is wide and pale yellow; heartwood is
dark orange. The wood is heavy, coarse grained, and resinous.
Shrinkage is moderately high. The wood is moderately
strong, stiff, moderately hard, and moderately high in shock
Pond pine is used for general construction, railway crossties,
posts, and poles. The lumber of this species is also graded
as a minor species in grading rules for the Southern Pine
Ponderosa pine (Pinus ponderosa) is also known as ponderosa,
western soft, western yellow, bull, and blackjack pine.
Jeffrey pine (P. jeffreyi), which grows in close association
with ponderosa pine in California and Oregon, is usually
marketed with ponderosa pine and sold under that name.
Major ponderosa pine producing areas are in Oregon, Washington,
and California (Fig. 1–3). Other important producing
areas are in Idaho and Montana; lesser amounts come from
the southern Rocky Mountain region, the Black Hills of
South Dakota, and Wyoming.
The heartwood of ponderosa pine is light reddish brown, and
the wide sapwood is nearly white to pale yellow. The wood
of the outer portions of ponderosa pine of sawtimber size is
generally moderately light in weight, moderately low in
strength, moderately soft, moderately stiff, and moderately
low in shock resistance. It is generally straight grained and
has moderately low shrinkage. It is quite uniform in texture
and has little tendency to warp and twist.
Ponderosa pine is used mainly for lumber and to a lesser
extent for piles, poles, posts, mine timbers, veneer, and
railroad crossties. The clear wood is used for sashes, doors,
blinds, moulding, paneling, interior woodwork, and built-in
cases and cabinets. Low-grade lumber is used for boxes and
crates. Much intermediate- or low-grade lumber is used for
sheathing, subflooring, and roof boards. Knotty ponderosa
pine is used for interior woodwork.
Figure 1–3. Ponderosa pine (Pinus ponderosa) growing
in an open or park-like habitat.
Red pine (Pinus resinosa) is frequently called Norway pine
and occasionally known as hard pine and pitch pine. This
species grows in New England, New York, Pennsylvania,
and the Great Lake States.
The heartwood of red pine varies from pale red to reddish
brown. The sapwood is nearly white with a yellowish tinge
and is generally from 5 to 10 cm (2 to 4 in.) wide. The
wood resembles the lighter weight wood of the Southern
Pine species group. Latewood is distinct in the growth rings.
Red pine is moderately heavy, moderately strong and stiff,
moderately soft, and moderately high in shock resistance. It
is generally straight grained, not as uniform in texture as
eastern white pine (Pinus strobus), and somewhat resinous.
The wood has moderately high shrinkage, but it is not
difficult to dry and is dimensionally stable when dried.
Red pine is used principally for lumber, cabin logs, and
pulpwood, and to a lesser extent for piles, poles, posts, and
fuel. The lumber is used for many of the same purposes as for
eastern white pine (Pinus strobus). Red pine lumber is used
primarily for building construction, including treated lumber
for decking, siding, flooring, sashes, doors, general millwork,
and boxes, pallets, and crates.
A number of species are included in the group marketed as
Southern Pine lumber. The four major Southern Pine species
and their growth ranges are as follows: (a) longleaf pine
(Pinus palustris), eastern North Carolina southward into
Florida and westward into eastern Texas; (b) shortleaf pine
(P. echinata), southeastern New York and New Jersey
southward to northern Florida and westward into eastern
Texas and Oklahoma; (c) loblolly pine (P. taeda), Maryland
southward through the Atlantic Coastal Plain and Piedmont
Plateau into Florida and westward into eastern Texas; (d)
slash pine (P. elliottii), Florida and southern South Carolina,
Georgia, Alabama, Mississippi, and Louisiana east of
the Mississippi River. Lumber from these four species is
classified as Southern Pine by the grading standards of the
industry. These standards also classify lumber produced from
the longleaf and slash pine species as longleaf pine if the
lumber conforms to the growth-ring and latewood requirements
of such standards. Southern Pine lumber is produced
principally in the Southern and South Atlantic States. Georgia,
Alabama, North Carolina, Arkansas, and Louisiana lead
in Southern Pine lumber production.
The wood of these southern pines is quite similar in appearance.
Sapwood is yellowish white and heartwood, reddish
brown. The sapwood is usually wide in second-growth
stands. The heartwood begins to form when the tree is about
20 years old. In old, slow-growth trees, sapwood may be
only 2 to 5 cm (1 to 2 in.) wide.
Longleaf and slash pine are classified as heavy, strong, stiff,
hard, and moderately high in shock resistance. Shortleaf and
loblolly pine are usually somewhat lighter in weight than is
longleaf. All the southern pines have moderately high
shrinkage but are dimensionally stable when properly dried.
To obtain heavy, strong wood of the southern pines for
structural purposes, a density rule has been written that
specifies a certain percentage of latewood and growth rates for
The denser and higher strength southern pines are extensively
used in the form of stringers in construction of factories,
warehouses, bridges, trestles, and docks, and also for
roof trusses, beams, posts, joists, and piles. Lumber of lower
density and strength is also used for building material, such
as interior woodwork, sheathing, and subflooring, as well as
boxes, pallets, and crates. Southern Pine is used also for
tight and slack cooperage. When used for railroad crossties,
piles, poles, mine timbers, and exterior decking, it is usually
treated with preservatives. The manufacture of structuralgrade
plywood from Southern Pine is a major wood-using
industry, as is the production of preservative-treated lumber.
Spruce pine (Pinus glabra), also known as cedar, poor,
Walter, and bottom white pine, is classified as a minor
species in the Southern Pine species group. Spruce pine
grows most commonly on low moist lands of the coastal
regions of southeastern South Carolina, Georgia, Alabama,
Mississippi, and Louisiana, and northern and northwestern
The heartwood of spruce pine is light brown, and the wide
sapwood is nearly white. Spruce pine wood is lower in most
strength values than the wood of the major Southern Pine
species group. Spruce pine compares favorably with the
western true firs in important bending properties, crushing
strength (perpendicular and parallel to grain), and hardness.
It is similar to denser species such as coast Douglas-fir
(Pseudotsuga menziesii) and loblolly pine (Pinus taeda)
in shear parallel to grain.
In the past, spruce pine was principally used locally for
lumber, pulpwood, and fuelwood. The lumber reportedly
was used for sashes, doors, and interior woodwork because
of its low specific gravity and similarity of earlywood and
latewood. In recent years, spruce pine has been used for
Sugar pine (Pinus lambertiana), the world’s largest species
of pine, is sometimes called California sugar pine. Most
sugar pine lumber grows in California and southwestern
The heartwood of sugar pine is buff or light brown, sometimes
tinged with red. The sapwood is creamy white. The
wood is straight grained, fairly uniform in texture, and easy
to work with tools. It has very low shrinkage, is readily
dried without warping or checking, and is dimensionally
stable. Sugar pine is lightweight, moderately low in
strength, moderately soft, low in shock resistance, and low
Sugar pine is used almost exclusively for lumber products.
The largest volume is used for boxes and crates, sashes,
doors, frames, blinds, general millwork, building construction,
and foundry patterns. Like eastern white pine (Pinus
strobus), sugar pine is suitable for use in nearly every part
of a house because of the ease with which it can be cut, its
dimensional stability, and its good nailing properties.
Virginia pine (Pinus virginiana), also known as Jersey and
scrub pine, grows from New Jersey and Virginia throughout
the Appalachian region to Georgia and the Ohio Valley.
It is classified as a minor species in the grading rules for
the Southern Pine species group.
The heartwood is orange, and the sapwood is nearly white
and relatively wide. The wood is moderately heavy, moderately
strong, moderately hard, and moderately stiff and has
moderately high shrinkage and high shock resistance.
Virginia pine is used for lumber, railroad crossties, mine
timbers, and pulpwood.
Pine, Western White
Western white pine (Pinus monticola) is also known as
Idaho white pine or white pine. About four-fifths of the wood
for lumber from this species is from Idaho and Washington;
small amounts are cut in Montana and Oregon.
The heartwood of western white pine is cream colored to
light reddish brown and darkens on exposure to air. The
sapwood is yellowish white and generally from 2 to 8 cm
(1 to 3 in.) wide. The wood is straight grained, easy to
work, easily kiln-dried, and stable after drying. This species
is moderately lightweight, moderately low in strength,
moderately soft, moderately stiff, and moderately low in
shock resistance and has moderately high shrinkage.
Practically all western white pine is sawn into lumber, which
is used mainly for building construction, matches, boxes,
patterns, and millwork products, such as sashes and door
frames. In building construction, lower-grade boards are used
for sheathing, knotty paneling, and subflooring. High-grade
material is made into siding of various kinds, exterior and
interior woodwork, and millwork. Western white pine has
practically the same uses as eastern white pine (Pinus
strobus) and sugar pine (Pinus lambertiana).
Port-Orford-cedar (Chamaecyparis lawsoniana) is sometimes
known as Lawson-cypress, Oregon-cedar, and white-cedar. It
grows along the Pacific Coast from Coos Bay, Oregon,
southward to California. It does not extend more than
64 km (40 mi) inland.
The heartwood of Port-Orford-cedar is light yellow to pale
brown. The sapwood is narrow and hard to distinguish from
the heartwood. The wood has fine texture, generally straight
grain, and a pleasant spicy odor. It is moderately lightweight,
stiff, moderately strong and hard, and moderately
resistant to shock. Port-Orford-cedar heartwood is highly
resistant to decay. The wood shrinks moderately, has little
tendency to warp, and is stable after drying.
Some high-grade Port-Orford-cedar was once used in the
manufacture of storage battery separators, matchsticks, and
specialty millwork. Today, other uses are archery supplies,
sash and door construction, stadium seats, flooring, interior
woodwork, furniture, and boats.
Eastern redcedar (Juniperus virginiana) grows throughout the
eastern half of the United States, except in Maine, Florida,
and a narrow strip along the Gulf Coast, and at the higher
elevations in the Appalachian Mountain Range. Commercial
production is principally in the southern Appalachian and
Cumberland Mountain regions. Another species, southern
redcedar (J. silicicola), grows over a limited area in the
South Atlantic and Gulf Coastal Plains.
The heartwood of redcedar is bright or dull red, and the
narrow sapwood is nearly white. The wood is moderately
heavy, moderately low in strength, hard, and high in shock
resistance, but low in stiffness. It has very low shrinkage and
is dimensionally stable after drying. The texture is fine and
uniform, and the wood commonly has numerous small
knots. Eastern redcedar heartwood is very resistant to decay.
The greatest quantity of eastern redcedar is used for fence
posts. Lumber is manufactured into chests, wardrobes, and
closet lining. Other uses include flooring, novelties, pencils,
scientific instruments, and small boats. Southern redcedar
is used for the same purposes. Eastern redcedar is reputed
to repel moths, but this claim has not been supported by
Western redcedar (Thuja plicata) grows in the Pacific
Northwest and along the Pacific Coast to Alaska. It is also
called canoe-cedar, giant arborvitae, shinglewood, and Pacific
redcedar. Western redcedar lumber is produced principally in
Washington, followed by Oregon, Idaho, and Montana.
The heartwood of western redcedar is reddish or pinkish
brown to dull brown, and the sapwood is nearly white. The
sapwood is narrow, often not more than 2.5 cm (1 in.) wide.
The wood is generally straight grained and has a uniform but
rather coarse texture. It has very low shrinkage. This species
is lightweight, moderately soft, low in strength when used as
a beam or posts, and low in shock resistance. The heartwood
is very resistant to decay.
Western redcedar is used principally for shingles, lumber,
poles, posts, and piles. The lumber is used for exterior
siding, decking, interior woodwork, greenhouse construction,
ship and boat building, boxes and crates, sashes,
Redwood (Sequoia sempervirens) grows on the coast of
California and some trees are among the tallest in the world.
A closely related species, giant sequoia (Sequoiadendron
giganteum), is volumetrically larger and grows in a limited
area in the Sierra Nevadas of California, but its wood is used
in very limited quantities. Other names for redwood are coast
redwood, California redwood, and sequoia. Production of
redwood lumber is limited to California, but the market is
The heartwood of redwood varies from light ―cherry‖ red to
dark mahogany. The narrow sapwood is almost white. Typical
old-growth redwood is moderately lightweight, moderately
strong and stiff, and moderately hard. The wood is easy
to work, generally straight grained, and shrinks and swells
comparatively little. The heartwood from old-growth trees
has high decay resistance; heartwood from second-growth
trees generally has low to moderate decay resistance.
Most redwood lumber is used for building. It is remanufactured
extensively into siding, sashes, doors, blinds, millwork,
casket stock, and containers. Because of its durability,
redwood is useful for cooling towers, decking, tanks, silos,
wood-stave pipe, and outdoor furniture. It is used in agriculture
for buildings and equipment. Its use as timbers and large
dimension in bridges and trestles is relatively minor. Redwood
splits readily and plays an important role in the
manufacture of split products, such as posts and fence
material. Some redwood veneer is produced for decorative
The term eastern spruce includes three species: red (Picea
rubens), white (P. glauca), and black (P. mariana). White
and black spruce grow principally in the Great Lake States
and New England, and red spruce grows in New England
and the Appalachian Mountains.
The wood is light in color, and there is little difference
between heartwood and sapwood. All three species have
about the same properties, and they are not distinguished
from each other in commerce. The wood dries easily and is
stable after drying, is moderately lightweight and easily
worked, has moderate shrinkage, and is moderately strong,
stiff, tough, and hard.
The greatest use of eastern spruce is for pulpwood. Eastern
spruce lumber is used for framing material, general millwork,
boxes and crates, and piano sounding boards.
Engelmann spruce (Picea engelmannii) grows at high elevations
in the Rocky Mountain region of the United States.
This species is also known as white spruce, mountain
spruce, Arizona spruce, silver spruce, and balsam. About
two-thirds of the lumber is produced in the southern Rocky
Mountain States and most of the remainder in the northern
Rocky Mountain States and Oregon.
The heartwood of Engelmann spruce is nearly white, with a
slight tinge of red. The sapwood varies from 2 to 5 cm
(3/4 to 2 in.) in width and is often difficult to distinguish
from the heartwood. The wood has medium to fine texture
and is without characteristic odor. Engelmann spruce is rated
as lightweight, and it is low in strength as a beam or post. It
is also soft and low in stiffness, shock resistance, and shrinkage.
The lumber typically contains many small knots.
Engelmann spruce is used principally for lumber and for
mine timbers, railroad crossties, and poles. It is used also in
building construction in the form of dimension lumber,
flooring, and sheathing. It has excellent properties for pulp
Sitka spruce (Picea sitchensis) is a large tree that grows
along the northwestern coast of North America from California
to Alaska. It is also known as yellow, tideland, western,
silver, and west coast spruce. Much Sitka spruce timber is
grown in Alaska, but most logs are sawn into cants for
export to Pacific Rim countries. Material for U.S. consumption
is produced primarily in Washington and Oregon.
The heartwood of Sitka spruce is a light pinkish brown. The
sapwood is creamy white and shades gradually into the
heartwood; the sapwood may be 7 to 15 cm (3 to 6 in.) wide
or even wider in young trees. The wood has a comparatively
fine, uniform texture, generally straight grain, and no distinct
taste or odor. It is moderately lightweight, moderately low
in bending and compressive strength, moderately stiff, moderately
soft, and moderately low in resistance to shock. It has
moderately low shrinkage. On the basis of weight, Sitka
spruce rates high in strength properties and can be obtained
in long, clear, straight-grained pieces.
Sitka spruce is used principally for lumber, pulpwood, and
cooperage. Boxes and crates account for a considerable
amount of the remanufactured lumber. Other important uses
are furniture, planing-mill products, sashes, doors, blinds,
millwork, and boats. Sitka spruce has been by far the most
important wood for aircraft construction. Other specialty uses
are ladder rails and sounding boards for pianos.
Tamarack (Larix laricina), also known as eastern larch and
locally as hackmatack, is a small to medium tree with a
straight, round, slightly tapered trunk. It grows from Maine
to Minnesota, with the bulk of the stand in the Great Lake
The heartwood of tamarack is yellowish brown to russet
brown. The sapwood is whitish, generally less than 2.5 cm
(1 in.) wide. The wood is coarse in texture, without odor or
taste, and the transition from earlywood to latewood is
abrupt. The wood is intermediate in weight and in most
Tamarack is used principally for pulpwood, lumber, railroad
crossties, mine timbers, fuel, fence posts, and poles. Lumber
is used for framing material, tank construction, and boxes,
pallets, and crates. The production of tamarack lumber has
declined in recent years.
White-Cedar, Northern and Atlantic
Two species of white-cedar grow in the eastern part of the
United States: northern white-cedar (Thuja occidentalis) and
Atlantic white-cedar (Chamaecyparis thyoides). Northern
white-cedar is also known as arborvitae or simply as cedar.
Atlantic white-cedar is also known as southern white-cedar,
swamp-cedar, and boat-cedar. Northern white-cedar grows
from Maine along the Appalachians and westward through
the northern part of the Great Lake States. Atlantic whitecedar
grows near the Atlantic Coast from Maine to northern
Florida and westward along the Gulf Coast to Louisiana. It
is strictly a swamp tree. Production of northern white-cedar
lumber is greatest in Maine and the Great Lake States. Production
of Atlantic white-cedar centers in North Carolina and
along the Gulf Coast.
The heartwood of white-cedar is light brown, and the sapwood
is white or nearly so. The sapwood is usually narrow.
The wood is lightweight, rather soft, and low in strength and
shock resistance. It shrinks little in drying. It is easily
worked and holds paint well, and the heartwood is highly
resistant to decay. Northern and Atlantic white-cedar are used
for similar purposes, primarily for poles, cabin logs, railroad
crossties, lumber, posts, and decorative fencing. White-cedar
lumber is used principally where a high degree of durability
is needed, as in tanks and boats, and for wooden ware.
Yellow-cedar (Chamaecyparis nootkatensis) grows in the
Pacific Coast region of North America from southeastern
Alaska southward through Washington to southern Oregon.
The heartwood of yellow-cedar is bright, clear yellow. The
sapwood is narrow, white to yellowish, and hardly distinguishable
from the heartwood. The wood is fine textured and
generally straight grained. It is moderately heavy, moderately
strong and stiff, moderately hard, and moderately high in
shock resistance. Yellow-cedar shrinks little in drying and is
stable after drying, and the heartwood is very resistant to
decay. The wood has a mild, distinctive odor.
Yellow-cedar is used for interior woodwork, furniture, small
boats, cabinetwork, and novelties.
This section does not purport to describe all the woods that
have been at one time or another imported into the United
States. It includes only those species that at present are
considered to be commercially important. The same species
may be marketed in the United States under other common
names. Because of the variation in common names, many
cross-references are included. Text information is necessarily
brief, but when used in conjunction with the shrinkage and
strength data tables (Ch. 3 and 4), a reasonably good picture
may be obtained of a particular wood. The references at the
end of this chapter contain information on many species not
described in this section.
Afara (see Limba)
Afrormosia or kokrodua (Pericopsis elata), a large West
African tree, is sometimes used as a substitute for teak
The heartwood is fine textured, with straight to interlocked
grain. The wood is brownish yellow with darker streaks and
moderately hard and heavy, weighing about 700 kg/m3
(43 lb/ft3) at 15% moisture content. The wood strongly
resembles teak in appearance but lacks its oily nature and has
a different texture. The wood dries readily with little degrade
and has good dimensional stability. It is somewhat heavier
and stronger than teak. The heartwood is highly resistant to
decay fungi and termite attack and is extremely durable under
Afrormosia is often used for the same purposes as teak, such
as boat construction, joinery, flooring, furniture, interior
woodwork, and decorative veneer.
Albarco, or jequitiba as it is known in Brazil, is the common
name applied to species in the genus Cariniana. The
10 species are distributed from eastern Peru and northern
Bolivia through central Brazil to Venezuela and Colombia.
The heartwood is reddish or purplish brown and sometimes
has dark streaks. It is usually not sharply demarcated from
the pale brown sapwood. The texture is medium and the
grain straight to interlocked. Albarco can be worked satisfactorily
with only slight blunting of tool cutting edges because
of the presence of silica. Veneer can be cut without difficulty.
The wood is rather strong and moderately heavy, weighing
about 560 kg/m3 (35 lb/ft3) at 12% moisture content. In
general, the wood has about the same strength as that of U.S.
oaks (Quercus spp.). The heartwood is durable, particularly
the deeply colored material. It has good resistance to drywood
Albarco is primarily used for general construction and carpentry
wood, but it can also be used for furniture components,
shipbuilding, flooring, veneer for plywood, and turnery.
Amaranth (see Purpleheart)
Anani (see Manni)
Anaura (see Marishballi)
Because of the widespread distribution of andiroba (Carapa
guianensis) in tropical America, the wood is known under a
variety of names, including cedro macho, carapa, crabwood,
and tangare. These names are also applied to the related
species Carapa nicaraguensis, whose properties are generally
inferior to those of C. guianensis.
The heartwood varies from medium to dark reddish brown.
The texture is like that of true mahogany (Swietenia macrophylla),
and andiroba is sometimes substituted for true mahogany.
The grain is usually interlocked but is rated easy to
work, paint, and glue. The wood is rated as durable to very
durable with respect to decay and insects. Andiroba is heavier
than true mahogany and accordingly is markedly superior
in all static bending properties, compression parallel to
grain, hardness, shear, and durability.
On the basis of its properties, andiroba appears to be suited
for such uses as flooring, frame construction in the tropics,
furniture and cabinetwork, millwork, utility and decorative
veneer, and plywood.
Angelin (see Sucupira)
Angelique (Dicorynia guianensis) comes from French
Guiana and Suriname.
Because of the variability in heartwood color between different
trees, two forms are commonly recognized by producers.
The heartwood that is russet-colored when freshly cut and
becomes superficially dull brown with a purplish cast is
referred to as ―gris.‖ The heartwood that is more distinctly
reddish and frequently shows wide purplish bands is called
―angelique rouge.‖ The texture of the wood is somewhat
coarser than that of black walnut (Juglans nigra), and the
grain is generally straight or slightly interlocked. In strength,
angelique is superior to teak (Tectona grandis) and white
oak (Quercus alba), when green or air dry, in all properties
except tension perpendicular to grain. Angelique is rated as
highly resistant to decay and resistant to marine borer attack.
Machining properties vary and may be due to differences in
density, moisture content, and silica content. After the wood
is thoroughly air or kiln dried, it can be worked effectively
only with carbide-tipped tools.
The strength and durability of angelique make it especially
suitable for heavy construction, harbor installations, bridges,
heavy planking for pier and platform decking, and railroad
bridge ties. The wood is also suitable for ship decking,
planking, boat frames, industrial flooring, and parquet blocks
Apa (see Wallaba)
Apamate (see Roble)
Apitong (see Keruing)
Avodire (Turraeanthus africanus) has a rather extensive
range in Africa, from Sierra Leone westward to the Congo
region and southward to Zaire and Angola. It is most common
in the eastern region of the Ivory Coast and is scattered
elsewhere. Avodire is a medium-size tree of the rainforest
where it forms fairly dense but localized and discontinuous
The wood is cream to pale yellow with high natural luster; it
eventually darkens to a golden yellow. The grain is sometimes
straight but more often wavy or irregularly interlocked,
which produces an unusual and attractive mottled figure
when sliced or cut on the quarter. Although avodire weighs
less than northern red oak (Quercus rubra), it has almost
identical strength properties except that it is lower in shock
resistance and shear. The wood works fairly easily with hand
and machine tools and finishes well in most operations.
Figured material is usually converted into veneer for use in
decorative work, and it is this kind of material that is chiefly
imported into the United States. Other uses include furniture,
fine joinery, cabinetwork, and paneling.
Azobe or ekki (Lophira alata) is found in West Africa and
extends into the Congo basin.
The heartwood is dark red, chocolate-brown, or purple–
brown with conspicuous white deposits in the pores
(vessels). The texture is coarse, and the grain is usually
interlocked. The wood is strong, and its density averages
about 1,120 kg/m3 (70 lb/ft3) at 12% moisture content. It is
very difficult to work with hand and machine tools, and tools
are severely blunted if the wood is machined when dry.
Azobe can be dressed to a smooth finish, and gluing properties
are usually good. Drying is very difficult without excessive
degrade. The heartwood is rated as very durable against
decay but only moderately resistant to termite attack. Azobe
is very resistant to acid and has good weathering properties.
It is also resistant to teredo attack. The heartwood is
extremely resistant to preservative treatment.
Azobe is excellent for heavy construction work, harbor construction,
heavy-duty flooring, and railroad crossties.
Bagtikan (see Seraya, White)
Balata or bulletwood (Manilkara bidentata) is widely distributed
throughout the West Indies, Central America, and
northern South America.
The heartwood of balata is light to dark reddish brown and
not sharply demarcated from the pale brown sapwood. Texture
is fine and uniform, and the grain is straight to occasionally
wavy or interlocked. Balata is a strong and very heavy
wood; density of air-dried wood is 1,060 kg/m3 (66 lb/ft3). It
is generally difficult to air dry, with a tendency to develop
severe checking and warp. The wood is moderately easy to
work despite its high density, and it is rated good to excellent
in all machining operations. Balata is very resistant to
attack by decay fungi and highly resistant to subterranean
termites but only moderately resistant to dry-wood termites.
Balata is suitable for heavy construction, textile and pulpmill
equipment, furniture parts, turnery, tool handles, flooring,
boat frames and other bentwork, railroad crossties, violin
bows, billiard cues, and other specialty uses.
Balau, red balau, and selangan batu constitute a group of
species that are the heaviest of the 200 Shorea species. About
45 species of this group grow from Sri Lanka and southern
India through southeast Asia to the Philippines.
The heartwood is light to deep red or purple–brown, and it
is fairly distinct from the lighter and yellowish- to reddishor
purplish-brown sapwood. The texture is moderately fine
to coarse, and the grain is often interlocked. The wood
weighs more than 750 kg/m3 (47 lb/ft3) at 12% moisture
content. Balau is a heavy, hard, and strong timber that dries
slowly with moderate to severe end checks and splits. The
heartwood is durable to moderately durable and very resistant
to preservative treatments.
Balau is used for heavy construction, frames of boats, decking,
flooring, and utility furniture.
Balau, Red (see Balau)
Balsa (Ochroma pyramidale) is widely distributed throughout
tropical America from southern Mexico to southern
Brazil and Bolivia, but Ecuador has been the principal source
of supply since the wood gained commercial importance. It
is usually found at lower elevations, especially on bottomland
soils along streams and in clearings and cutover forests.
Today, it is often cultivated in plantations.
Several characteristics make balsa suitable for a wide variety
of uses. It is the lightest and softest of all woods on the
market. The lumber selected for use in the United States
weighs, on the average, about 180 kg/m3 (11 lb/ft3) when dry
and often as little as 100 kg/m3 (6 lb/ft3). The wood is readily
recognized by its light weight; nearly white or oatmeal
color, often with a yellowish or pinkish hue; and unique
Because of its light weight and exceedingly porous composition,
balsa is highly efficient in uses where buoyancy, insulation
against heat or cold, or low propagation of sound and
vibration are important. Principal uses are for life-saving
equipment, floats, rafts, corestock, insulation, cushioning,
sound modifiers, models, and novelties.
Various species of banak (Virola) occur in tropical America,
from Belize and Guatemala southward to Venezuela, the
Guianas, the Amazon region of northern Brazil, and southern
Brazil, and on the Pacific Coast to Peru and Bolivia. Most of
the wood known as banak is V. koschnyi of Central America
and V. surinamensis and V. sebifera of northern South
America. Botanically, cuangare (Dialyanthera) is closely
related to banak, and the woods are so similar that they are
generally mixed in the trade. The main commercial supply of
cuangare comes from Colombia and Ecuador. Banak and
cuangare are common in swamp and marsh forests and may
occur in almost pure stands in some areas.
The heartwood of both banak and cuangare is usually pinkish
or grayish brown and is generally not differentiated from the
sapwood. The wood is straight grained and is of a medium
to coarse texture. The various species are nonresistant to
decay and insect attack but can be readily treated with preservatives.
Machining properties are very good, but when
zones of tension wood are present, machining may result in
surface fuzziness. The wood finishes readily and is easily
glued. Strength properties of banak and cuangare are similar
to those of yellow-poplar (Liriodendron tulipifera).
Banak is considered a general utility wood for lumber, veneer,
and plywood. It is also used for moulding, millwork,
and furniture components.
Benge (Ehie, Bubinga)
Although benge (Guibourtia arnoldiana), ehie or ovangkol
(Guibourtia ehie), and bubinga (Guibourtia spp.) belong to
the same West African genus, they differ rather markedly in
color and somewhat in texture.
The heartwood of benge is pale yellowish brown to medium
brown with gray to almost black stripes. Ehie heartwood
tends to be more golden brown to dark brown with gray to
almost black stripes. Bubinga heartwood is pink, vivid red,
or red–brown with purple streaks, and it becomes yellow or
medium brown with a reddish tint upon exposure to air. The
texture of ehie is moderately coarse, whereas that of benge
and bubinga is fine to moderately fine. All three woods are
moderately hard and heavy, but they can be worked well
with hand and machine tools. They are listed as moderately
durable and resistant to preservative treatment. Drying may
be difficult, but with care, the wood dries well.
These woods are used in turnery, flooring, furniture components,
cabinetwork, and decorative veneers.
Brown Silverballi (see Kaneelhart)
Bubinga (see Benge)
Bulletwood (see Balata)
Carapa (see Andiroba)
Cativo (Prioria copaifera) is one of the few tropical American
species that occur in abundance and often in nearly pure
stands. Commercial stands are found in Nicaragua, Costa
Rica, Panama, and Colombia.
Sapwood may be very pale pink or distinctly reddish, and it
is usually wide. In trees up to 76 cm (30 in.) in diameter,
heartwood may be only 18 cm (7 in.) in diameter. The grain
is straight and the texture of the wood is uniform, comparable
with that of true mahogany (Swietenia macrophylla). On
flat-sawn surfaces, the figure is rather subdued as a result of
exposure of the narrow bands of parenchyma tissue. The
wood can be dried rapidly and easily with very little degrade.
Dimensional stability is very good—practically equal to that
of true mahogany. Cativo is classified as a nondurable wood
with respect to decay and insects. It may contain appreciable
quantities of gum. In wood that has been properly dried,
however, the aromatics in the gum are removed and there is
no difficulty in finishing.
Considerable quantities of cativo are used for interior woodwork,
and resin-stabilized veneer is an important pattern
material. Cativo is widely used for furniture and cabinet
parts, lumber core for plywood, picture frames, edge banding
for doors, joinery, and millwork.
Cedro (see Spanish-Cedar)
Cedro Macho (see Andiroba)
Cedro-Rana (see Tornillo)
Ceiba (Ceiba pentandra) is a large tree, which grows to
66 m (200 ft) in height with a straight cylindrical bole 13 to
20 m (40 to 60 ft) long. Trunk diameters of 2 m (6 ft) or
more are common. Ceiba grows in West Africa, from the
Ivory Coast and Sierra Leone to Liberia, Nigeria, and the
Congo region. A related species is lupuna (Ceiba samauma)
from South America.
Sapwood and heartwood are not clearly demarcated. The
wood is whitish, pale brown, or pinkish brown, often with
yellowish or grayish streaks. The texture is coarse, and the
grain is interlocked or occasionally irregular. Ceiba is very
soft and light; density of air-dried wood is 320 kg/m3
(20 lb/ft3). In strength, the wood is comparable with basswood
(Tilia americana). Ceiba dries rapidly without marked
deterioration. It is difficult to saw cleanly and dress smoothly
because of the high percentage of tension wood. It provides
good veneer and is easy to nail and glue. Ceiba is very
susceptible to attack by decay fungi and insects. It requires
rapid harvest and conversion to prevent deterioration. Treatability,
however, is rated as good.
Ceiba is available in large sizes, and its low density combined
with a rather high degree of dimensional stability make
it ideal for pattern and corestock. Other uses include blockboard,
boxes and crates, joinery, and furniture components.
Chewstick (see Manni)
The genus Hymenaea consists of about 25 species that occur
in the West Indies and from southern Mexico through Central
America into the Amazon basin of South America. The
best-known and most important species is H. courbaril,
which occurs throughout the range of the genus. Courbaril is
often called jatoba in Brazil.
Sapwood of courbaril is gray–white and usually quite wide.
The heartwood, which is sharply differentiated from the
sapwood, is salmon red to orange–brown when freshly cut
and becomes russet or reddish brown when dried. The heartwood
is often marked with dark streaks. The texture is medium
to rather coarse, and the grain is mostly interlocked.
The wood is hard and heavy (about 800 kg/m3 (50 lb/ft3) at
12% moisture content). The strength properties of courbaril
are quite high and very similar to those of shagbark hickory
(Carya ovata), a species of lower specific gravity. Courbaril
is rated as moderately to very resistant to attack by decay
fungi and dry-wood termites. The heartwood is not treatable,
but the sapwood is treatable with preservatives. Courbaril is
moderately difficult to saw and machine because of its high
density, but it can be machined to a smooth surface. Turning,
gluing, and finishing properties are satisfactory. Planing,
however, is somewhat difficult because of the interlocked
grain. Courbaril compares favorably with white oak (Quercus
alba) in steam bending behavior.
Courbaril is used for tool handles and other applications that
require good shock resistance. It is also used for steam-bent